Transcript Full Depth Reclamation with Cement Presentation
Metropolitan Government Pavement Engineers Council
Full-Depth Reclamation with Cement
Full-Depth Reclamation with Cement Course Instructor: Don A. Clem, P.E.
Executive Director Portland Cement Association Northwest & Rocky Mountain Region
Introduction Applications Benefits Design Construction Field Testing Performance
Cement-Based Pavement Materials
Roller-Compacted Concrete Pervious Concrete Conventional Concrete Soil-Cement Cement Treated Base Full-Depth Reclamation Cement-Modified Soil Water Content Flowable Fill
Concrete Soil-Cement Cementitious Gel or Paste coats all particles fills voids Hydration Products all particles not coated voids not filled linkages bind soil agglomerations together
Definition of Full-Depth Reclamation Method of flexible pavement reconstruction that utilizes the existing asphalt, base, and subgrade material to produce a new stabilized base course for a chip seal, asphalt, or concrete wearing surface.
Types of Reclamation Methods Mechanical Stabilization Bituminous Stabilization – emulsified asphalt – expanded (foamed) asphalt Chemical Stabilization portland cement slag cement fly ash kiln dust lime other
Surfaced Roadways in the United States (2,495,000 total centerline miles) Rigid
Challenges Facing Our Roadways Continuing growth Rising expectations from users A heavily used, aging system Environmental compatibility Changes in the workforce Funding limitations
Combined with large increases in traffic volumes and/or allowable loads often leads to serious roadway base failures!
How do you know if you have a base problem and not just a surface deficiency?
Examples of Pavement Distress Alligator cracking Rutting Excessive patching Base failures Potholes Soil stains on surface
Advantages of the FDR Process Use of in-place materials Little or no material hauled off and dumped Maintains or improves existing grade Conserves virgin material Saves cost by using in-place “investment” Saves energy by reducing mining and hauls Very sustainable process
Benefits of FDR with Cement Increased rigidity spreads loads Eliminates rutting below surface Reduced moisture susceptibility Reduced fatigue cracking in asphalt surfacing Allows for thinner pavement section
Rehabilitation Strategies Rehabilitation Strategy
New pavement structure Fast construction Minimal traffic disruption Minimal material in/out Conserves resources Maintains existing elevation Low cost
Reclamation with Cement
X X X X X Removal and Replacement
X X X X
Sustainable Element of FDR Process 12 180 4,500 300 2,700 0 3,000 500 1 mile of 24-foot wide, 2-lane road, with a 6-inch base
Pavement Thickness Design Procedures 1993 AASHTO Pavement Design Guide – Structural Numbers – Layer Coefficients Proposed New AASHTO Design Guide – – Mechanistic-Empirical Design Evaluates effects of pavement materials, traffic loading conditions, environmental factors, design features, and construction practices
Pavement Materials Tests Sieve Analysis (ASTM C136) Atterberg Limits (ASTM D4318) Moisture-Density (ASTM D558) Durability Tests – – Wet-Dry (ASTM D559) Freeze-Thaw (ASTM D560) Soluble Sulfates (ASTM C1580) Compressive Strength (ASTM D1633)
Laboratory Mix Design Obtain representative samples of roadway material Usually about 100 pounds of material is required Determine the maximum dry density and optimum moisture content at various cement percentages (ASTM D558) Typical designs vary between 2 and 8 percent cement by weight of dry material Prepare samples Cure samples
Strength Determination Unconfined Compressive Strength Testing ASTM D1633 Used by most governing agencies Simple and quick procedure 7-day strengths ranging from 300 to 400 psi are generally recommended Proven strength (support) under extremely heavy traffic conditions Proven performance (durability) in wet-dry and freeze-thaw environments
Please keep in mind that strength and performance are NOT the same thing!
The purpose of the mix design procedure is to select the correct amount of stabilizer that most closely balances both strength AND performance for the roadway materials!
FDR Construction Process Pulverize, Shape, Add Cement, Mix In Place, Compact, and Surface
New Surfacing Pulverized Pulverized
Stabilized Stabilized Subgrade Existing road Subgrade Subgrade Subgrade Subgrade Pulverization to desired depth Removal of excess material (if necessary) and shaping Addition of cement, mixing, reshaping, and compaction Final surface application
Inside a Reclaimer
Pulverization Pulverize mat to appropriate gradation Usually, only one pass is required!
Cement Spreading Cement is spread on top of the pulverized material in a measured amount in either a dry or slurry form
Blending of Materials and Moisture Addition Cement is blended into pulverized, reclaimed material and, with the addition of water, is brought to optimum moisture
Compaction and Grading Material is compacted to 96 to 98 percent minimum standard Proctor density and then graded to appropriate Plan lines, grades, and cross-sections
Curing Bituminous Compounds (cutbacks or emulsions) Water (kept continuously moist)
Testing Requirements Gradation/Uniformity Density Moisture A common gradation requirement is for 100 percent to pass a 3-inch sieve, a minimum of 95 percent to pass a 2-inch sieve, and a minimum of 55 percent to pass a No. 4 sieve (ASTM C136).
A common density requirement is to be between 96 and 98 percent of the established laboratory standard Proctor density (ASTM D558).
A common moisture requirement is to be within 2 percent of the laboratory established optimum moisture content (ASTM D558).
Traffic and Surfacing Completed FDR base can be opened immediately to low-speed local traffic and to construction equipment Subsequent pavement layers can be placed at any time
Laramie County, Wyoming Started using FDR for county roads in 2007
Little Sahara Rec Area 60,000 acres in south central Utah Reclaimed over 14 miles of park road Decision to use cement over another stabilizer saved $350,000
Richland County, Montana Just completed third year of FDR of chip seal and gravel roads Cement content developed for each road reclaimed More details by Steve Monlux, PE, LVR upcoming
Spanish Fork, Utah Two block long reconstruction project FDR process with cement saved $33,000 (21%) over conventional reconstruction Used micro-cracking Used the “Coyle” spreader
Counties who have purchased reclamers Weld County, Colorado Montrose County, Colorado
PCA Funded Project Study conducted in 2005 Identified candidate project sites in concert with PCA – State (DOT), County, City Agencies, Private Interaction with select officials Visual Pavement Condition Index (PCI) survey Extracted roadway cores for UCS measurements
79 Projects Studied Average = 9 years
LTP Study Conclusions Overall, excellent LTP Average PCI of 89 UCS of cores 260 to over 1,000 psi Cement contents 2 to 12 percent with average being 5 percent Most surface distress was in the asphalt layer No major failures attributed to the cement-stabilized base Owners are happy with performance and plan to do more in the future
Concluding Comments Use of in-place materials Very sustainable process Fast operation Constructed under traffic Structurally better than granular base Can apply local traffic almost immediately 30 to 60 percent less expensive than removal and replacement
For more on full-depth reclamation, visit the PCA website at www.cement.org/pavements
For further information please contact: Don A. Clem, PE [email protected]